General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.9 - 7.93 g/cm³ Show Material materials with Density of 7.9 - 7.93 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | -100.0 °C | 206 GPa Show Material materials with Elastic modulus of 206 GPa | |

20.0 °C | 196 - 200 GPa Show Material materials with Elastic modulus of 196 - 200 GPa | ||

100.0 °C | 190 GPa Show Material materials with Elastic modulus of 190 GPa | ||

200.0 °C | 182 - 185 GPa Show Material materials with Elastic modulus of 182 - 185 GPa | ||

300.0 °C | 174 - 175 GPa Show Material materials with Elastic modulus of 174 - 175 GPa | ||

400.0 °C | 166 - 170 GPa Show Material materials with Elastic modulus of 166 - 170 GPa | ||

500.0 °C | 158 - 160 GPa Show Material materials with Elastic modulus of 158 - 160 GPa | ||

600.0 °C | 150 - 155 GPa Show Material materials with Elastic modulus of 150 - 155 GPa | ||

700.0 °C | 142 - 145 GPa Show Material materials with Elastic modulus of 142 - 145 GPa | ||

800.0 °C | 134 - 140 GPa Show Material materials with Elastic modulus of 134 - 140 GPa | ||

900.0 °C | 127 - 135 GPa Show Material materials with Elastic modulus of 127 - 135 GPa | ||

1000.0 °C | 120 - 125 GPa Show Material materials with Elastic modulus of 120 - 125 GPa | ||

Elongation A80, transverse | 20.0 °C | 40 % Show Material materials with Elongation A80, transverse of 40 % | |

Elongation, transverse | 20.0 °C | 40 % Show Material materials with Elongation, transverse of 40 % | |

Poisson's ratio | 23.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | Typical for Austenitic Stainless Steel |

Shear modulus | 23.0 °C | 77 GPa Show Material materials with Shear modulus of 77 GPa | Typical for Austenitic Stainless Steel |

Tensile strength | 20.0 °C | 490 - 710 MPa Show Material materials with Tensile strength of 490 - 710 MPa | |

50.0 °C | 460 MPa Show Material materials with Tensile strength of 460 MPa | ||

100.0 °C | 410 MPa Show Material materials with Tensile strength of 410 MPa | ||

150.0 °C | 390 MPa Show Material materials with Tensile strength of 390 MPa | ||

200.0 °C | 370 MPa Show Material materials with Tensile strength of 370 MPa | ||

250.0 °C | 360 MPa Show Material materials with Tensile strength of 360 MPa | ||

300.0 °C | 350 MPa Show Material materials with Tensile strength of 350 MPa | ||

350.0 °C | 345 MPa Show Material materials with Tensile strength of 345 MPa | ||

400.0 °C | 340 MPa Show Material materials with Tensile strength of 340 MPa | ||

450.0 °C | 335 MPa Show Material materials with Tensile strength of 335 MPa | ||

500.0 °C | 330 MPa Show Material materials with Tensile strength of 330 MPa | ||

550.0 °C | 320 MPa Show Material materials with Tensile strength of 320 MPa | ||

600.0 °C | 300 MPa Show Material materials with Tensile strength of 300 MPa | ||

Unlock all property charts | |||

Tensile strength, transverse | 20.0 °C | 490 - 710 MPa Show Material materials with Tensile strength, transverse of 490 - 710 MPa | |

Yield strength Rp0.2 | 50.0 °C | 186 MPa Show Material materials with Yield strength Rp0.2 of 186 MPa | |

100.0 °C | 162 MPa Show Material materials with Yield strength Rp0.2 of 162 MPa | ||

150.0 °C | 152 MPa Show Material materials with Yield strength Rp0.2 of 152 MPa | ||

200.0 °C | 142 MPa Show Material materials with Yield strength Rp0.2 of 142 MPa | ||

250.0 °C | 137 MPa Show Material materials with Yield strength Rp0.2 of 137 MPa | ||

300.0 °C | 132 MPa Show Material materials with Yield strength Rp0.2 of 132 MPa | ||

350.0 °C | 127 MPa Show Material materials with Yield strength Rp0.2 of 127 MPa | ||

400.0 °C | 123 MPa Show Material materials with Yield strength Rp0.2 of 123 MPa | ||

450.0 °C | 118 MPa Show Material materials with Yield strength Rp0.2 of 118 MPa | ||

500.0 °C | 113 MPa Show Material materials with Yield strength Rp0.2 of 113 MPa | ||

550.0 °C | 108 MPa Show Material materials with Yield strength Rp0.2 of 108 MPa | ||

600.0 °C | 103 MPa Show Material materials with Yield strength Rp0.2 of 103 MPa | ||

Unlock all property charts | |||

Yield strength Rp0.2, transverse | 20.0 °C | 200 - 220 MPa Show Material materials with Yield strength Rp0.2, transverse of 200 - 220 MPa | |

Yield strength Rp1.0 | 50.0 °C | 225 MPa Show Material materials with Yield strength Rp1.0 of 225 MPa | |

100.0 °C | 201 MPa Show Material materials with Yield strength Rp1.0 of 201 MPa | ||

150.0 °C | 191 MPa Show Material materials with Yield strength Rp1.0 of 191 MPa | ||

200.0 °C | 181 MPa Show Material materials with Yield strength Rp1.0 of 181 MPa | ||

250.0 °C | 176 MPa Show Material materials with Yield strength Rp1.0 of 176 MPa | ||

300.0 °C | 172 MPa Show Material materials with Yield strength Rp1.0 of 172 MPa | ||

350.0 °C | 167 MPa Show Material materials with Yield strength Rp1.0 of 167 MPa | ||

400.0 °C | 162 MPa Show Material materials with Yield strength Rp1.0 of 162 MPa | ||

450.0 °C | 157 MPa Show Material materials with Yield strength Rp1.0 of 157 MPa | ||

500.0 °C | 152 MPa Show Material materials with Yield strength Rp1.0 of 152 MPa | ||

550.0 °C | 147 MPa Show Material materials with Yield strength Rp1.0 of 147 MPa | ||

600.0 °C | 142 MPa Show Material materials with Yield strength Rp1.0 of 142 MPa | ||

Unlock all property charts | |||

Yield strength Rp1.0, transverse | 20.0 °C | 240 - 250 MPa Show Material materials with Yield strength Rp1.0, transverse of 240 - 250 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | |

20.0 °C | 1.61E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 1/K | ||

100.0 °C | 1.63E-5 - 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.63E-5 - 1.67E-5 1/K | ||

200.0 °C | 1.69E-5 - 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.69E-5 - 1.72E-5 1/K | ||

300.0 °C | 1.73E-5 - 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.73E-5 - 1.77E-5 1/K | ||

400.0 °C | 1.78E-5 - 1.81E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.78E-5 - 1.81E-5 1/K | ||

500.0 °C | 1.82E-5 - 1.84E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.82E-5 - 1.84E-5 1/K | ||

600.0 °C | 1.85E-5 - 1.88E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.85E-5 - 1.88E-5 1/K | ||

700.0 °C | 1.87E-5 - 1.91E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.87E-5 - 1.91E-5 1/K | ||

800.0 °C | 1.94E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.94E-5 1/K | ||

900.0 °C | 1.97E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.97E-5 1/K | ||

1000.0 °C | 2E-5 1/K Show Material materials with Coefficient of thermal expansion of 2E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | -100.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

20.0 °C | 450 - 472 J/(kg·K) Show Material materials with Specific heat capacity of 450 - 472 J/(kg·K) | ||

100.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

200.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

300.0 °C | 512 J/(kg·K) Show Material materials with Specific heat capacity of 512 J/(kg·K) | ||

400.0 °C | 520 J/(kg·K) Show Material materials with Specific heat capacity of 520 J/(kg·K) | ||

500.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

600.0 °C | 541 J/(kg·K) Show Material materials with Specific heat capacity of 541 J/(kg·K) | ||

700.0 °C | 551 J/(kg·K) Show Material materials with Specific heat capacity of 551 J/(kg·K) | ||

800.0 °C | 559 J/(kg·K) Show Material materials with Specific heat capacity of 559 J/(kg·K) | ||

900.0 °C | 565 J/(kg·K) Show Material materials with Specific heat capacity of 565 J/(kg·K) | ||

1000.0 °C | 571 J/(kg·K) Show Material materials with Specific heat capacity of 571 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 14.3 - 17 W/(m·K) Show Material materials with Thermal conductivity of 14.3 - 17 W/(m·K) | |

100.0 °C | 15.8 W/(m·K) Show Material materials with Thermal conductivity of 15.8 W/(m·K) | ||

200.0 °C | 17.5 W/(m·K) Show Material materials with Thermal conductivity of 17.5 W/(m·K) | ||

300.0 °C | 19 W/(m·K) Show Material materials with Thermal conductivity of 19 W/(m·K) | ||

400.0 °C | 20.5 W/(m·K) Show Material materials with Thermal conductivity of 20.5 W/(m·K) | ||

500.0 °C | 21.9 W/(m·K) Show Material materials with Thermal conductivity of 21.9 W/(m·K) | ||

600.0 °C | 23.3 W/(m·K) Show Material materials with Thermal conductivity of 23.3 W/(m·K) | ||

700.0 °C | 24.6 W/(m·K) Show Material materials with Thermal conductivity of 24.6 W/(m·K) | ||

800.0 °C | 26 W/(m·K) Show Material materials with Thermal conductivity of 26 W/(m·K) | ||

900.0 °C | 27.4 W/(m·K) Show Material materials with Thermal conductivity of 27.4 W/(m·K) | ||

1000.0 °C | 28.8 W/(m·K) Show Material materials with Thermal conductivity of 28.8 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 3.8 mm²/s Show Material materials with Thermal diffusivity of 3.8 mm²/s | |

100.0 °C | 4 mm²/s Show Material materials with Thermal diffusivity of 4 mm²/s | ||

200.0 °C | 4.2 mm²/s Show Material materials with Thermal diffusivity of 4.2 mm²/s | ||

300.0 °C | 4.6 mm²/s Show Material materials with Thermal diffusivity of 4.6 mm²/s | ||

400.0 °C | 4.8 mm²/s Show Material materials with Thermal diffusivity of 4.8 mm²/s | ||

500.0 °C | 4.9 mm²/s Show Material materials with Thermal diffusivity of 4.9 mm²/s | ||

600.0 °C | 5 mm²/s Show Material materials with Thermal diffusivity of 5 mm²/s | ||

700.0 °C | 5.3 mm²/s Show Material materials with Thermal diffusivity of 5.3 mm²/s | ||

800.0 °C | 5.6 mm²/s Show Material materials with Thermal diffusivity of 5.6 mm²/s | ||

900.0 °C | 5.9 mm²/s Show Material materials with Thermal diffusivity of 5.9 mm²/s | ||

1000.0 °C | 6 mm²/s Show Material materials with Thermal diffusivity of 6 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 7.1E-7 Ω·m Show Material materials with Electrical resistivity of 7.1E-7 Ω·m |

100.0 °C | 7.76E-7 Ω·m Show Material materials with Electrical resistivity of 7.76E-7 Ω·m | |

200.0 °C | 8.49E-7 Ω·m Show Material materials with Electrical resistivity of 8.49E-7 Ω·m | |

300.0 °C | 9.14E-7 Ω·m Show Material materials with Electrical resistivity of 9.14E-7 Ω·m | |

400.0 °C | 9.71E-7 Ω·m Show Material materials with Electrical resistivity of 9.71E-7 Ω·m | |

500.0 °C | 1.02E-6 Ω·m Show Material materials with Electrical resistivity of 1.02E-6 Ω·m | |

600.0 °C | 1.07E-6 Ω·m Show Material materials with Electrical resistivity of 1.07E-6 Ω·m | |

700.0 °C | 1.1E-6 Ω·m Show Material materials with Electrical resistivity of 1.1E-6 Ω·m | |

800.0 °C | 1.14E-6 Ω·m Show Material materials with Electrical resistivity of 1.14E-6 Ω·m | |

900.0 °C | 1.17E-6 Ω·m Show Material materials with Electrical resistivity of 1.17E-6 Ω·m | |

1000.0 °C | 1.19E-6 Ω·m Show Material materials with Electrical resistivity of 1.19E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Boron | 1.5E-3 - 5E-3 % Show Material materials with Boron of 1.5E-3 - 5E-3 % |

Carbon | 0.04 - 0.08 % Show Material materials with Carbon of 0.04 - 0.08 % |

Chromium | 17 - 19 % Show Material materials with Chromium of 17 - 19 % |

Manganese | 2 % Show Material materials with Manganese of 2 % |

Nickel | 9 - 12 % Show Material materials with Nickel of 9 - 12 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |

Titanium | 0.8 % Show Material materials with Titanium of 0.8 % |